# PREDICTION OF WELD BEAD PENETRATION FOR STEEL USIN

```Shahnwaz Alam et al. / International Journal of Engineering Science and Technology (IJEST)
PENETRATION FOR STEEL USING
SUBMERGED ARC WELDING
PROCESS PARAMETERS
SHAHNWAZ ALAM
Department of Mechanical Engg. Integral University, Lucknow, India
sfzsa@rediffmail.com
DR.M.I.KHAN
Department of Mechanical Engg. Integral University, Lucknow, India
mikyh_20@yahoo.com
Abstract:
In these research paper the Design of experiment using 2-level full factorial technique has been used to conduct
experiments and to develop relationships mathematical models for predicting the weld bead penetration in
single wire submerged arc welding of 12 mm thick mild steel plates . The response factor, namely bead
penetration, as affected by arc voltage, current, welding speed, wire feed rate and nozzle-to-plate distance have
been investigated and analyzed.. The models developed have been checked for their adequacy and significance
by using the analysis of variance, F-test and the t-test, respectively. Main and interaction effects of the process
variables on weld bead penetration have also been presented in graphical form. The developed models could be
used for the prediction of important weld bead penetration and control of the weld bead quality by selecting
appropriate process parameter values. And the model-predicted penetration values have been compared with
their respective experimental values.
Keywords: Submerged arc welding, welding process parameters, Weld bead penetration, Mathematical
modelling and full factorial technique.
1. Introduction
Submerged arc welding as arc welding in which a continuous consumable electrode is used and the arc is
submerged in a granulated flux, some of which fuses to form a removable covering of slag on the weld. It is one
of the main welding processes used in the industries for the purpose of fabrication of huge structures is
Submerged Arc Welding process. The key features of this process are high deposition rates and long weld runs.
The important process variables in submerged arc welding are: welding current, arc voltage, welding speed,
nozzle to plate distance and wire feed rate. The effects of these process variables are determined through their
effects on weld bead penetration. Submerged arc welding is widely employed as one of the major fabrication
processes in industries to-day due to its inherent advantages of deep penetration, smooth bead, superior joint
quality, speed excellent weld appearance (without spatter) and high utilisation of electrode feed wire. It is one
of the oldest automatic welding processes introduced during 1930s.1,2,3 In SAW, researchers are often faced
with the problems of relating the process variables and bead geometry to the weld bead quality because there are
some unknown, nonlinear process parameters4 .Many efforts have been made to develop a mathematical model
to study these relationships and best way to solve this problem is by using experimental model .A multiple
regression technique has been utilized to establish the models for various welding processes 5,6 .R.S. Chandel
et al.7 presented theoretical predictions of the effect of current, electrode polarity, electrode diameter and
electrode extension on the melting rate, bead height, bead width and weld penetration. Datta et al. 8 proposed
multiple regression model for predicting volume of submerged arc deposit per unit time.Gupta V.K&amp; Pramar 9
used fractional factorial technique to predict geometric dimensions of the weld bead in SAW.Ravindra &amp;
Pramar 10 used a mathematical model to predict weld bead geometry for the flux cored welding process.
ISSN : 0975-5462
Vol. 3 No.10 October 2011
7408
Shahnwaz Alam et al. / International Journal of Engineering Science and Technology (IJEST)
Fig.-1 Experimental Set- up
2.
Plan of investigation.
2.1. Identification of important parameters
Review of literature and a large number of trial runs indicate that the dominant factors which are having
greater influence on the responses are open circuit voltage (OCV), welding current (I) , wire feed rate (F),
welding speed (S) and nozzle- to- plate distance (C) (15).
2.2. Determining the working limits of the parameters
Extensive trial runs have been carried out to find out the feasible working limits of submerged arc welding
parameters on mild steel. Different combinations of open circuit voltage (OCV), welding current (I) wire feed
rate (F), welding speed (S) and nozzle- to- plate distance (C) were used to observe the effect on desired
response. The weld zones were inspected with visual inspection to identify the working limits of the welding
parameters.
2.3. Developing the experimental design matrix
The feasible limits of the parameters were selected in such a way that the welds obtained were free from surface
defects. A two level full factorial design of (25-1 = 32) thirty two experimental runs, which is a standard
statistical tool to investigate the effects of number of parameters on the required response, was selected for
determining the effect of five independent direct welding parameters. This technique reduces the costs and
provides the required information about the main and interaction effects. The commonly employed method of
varying one parameter at a time, though popular, does not give any information about interaction among
parameters. Table -1 presents the working range of factors considered. For the convenience of the recording and
processing the experimental data the upper and lower levels of the factors are coded as -1 and +1 respectively.
2.4. Conducting the experiments as per designed matrix
The experiments were conducted at welding research division, RDSO (Research design and standard
organization Lucknow (U.P) India. The experiments have been performed on constant voltage fully automatic
submerged arc welding machine of a constant potential transformer-rectifier type (ESAB) with a maximum
welding current of 1000-1200 Amp. Experimental set-up shown in Fig.1.A 3.2mm copper coated mild steel feed
ISSN : 0975-5462
Vol. 3 No.10 October 2011
7409
Shahnwaz Alam et al. / International Journal of Engineering Science and Technology (IJEST)
wire electrode was used with composition of, (C-0.10%, Mn-0.45%, Si-0.02%). Welding was carried out in
single pass using bead on- plate technique. Weld beads were deposited according to the conditions directed by
the design matrix using 2- level 25-1 full factorial technique as given in table.2. The signs under the columns 1, 2,
3, 4 were arranged in standard full factorial order, while those other columns were obtained by taking treatment
product of parameters. A standard procedure was followed for designing such a matrix. The plates were cleaned
mechanically and chemically so as to remove oxide layer or any other sources of impurities, before welding.
The experiments were performed in a random order in order to avoid any systematic error. In 32 trials, beads
were laid on 32 plates. Two specimens of 16mm width were cut transverse to the welding direction from each
welded plates. These specimens were cleaned, ground, polished and etched with 10% nital (90% alcohol + 10%
of nitric acid). All specimens of first set were macro etched to reveal the bead profile and some specimens of
second set were micro etched to reveal the microstructures. Weld bead profiles were traced by using an optical
profile projector/Image at 20X magnification and the magnified view was drawn on the transparencies for
further analysis. Measurements were made for bead penetration (P). The observed values of the responses are
given in table.3.
2.4.1. Base Metal
Test specimens were prepared from 12 mm thickness Mild steel plate, 295x145x12mm size with a composition
of (C-0.102%,S-0.179%,Mn-0.466%,S-0.0705%,Cr-0.036%,Ni-0.022%).
2.4.2. Flux used
The study was carried out by using the available agglomerated flux, automelt GR-4 with a composition of (C0.08%, Mn-1.00%, Sn-0.25%).
Table1. Important process control variables
S.no
1
2
3
4
5
Parameters
Units
Notations
High (+1)
Low (-1)
Voltage
volts
V
35
29
Current
amp
I
550
400
Wire feed rate
Mm/min
F
3400
1600
Welding speed
Mm/min
S
600
360
Nozzle to plate mm
C
30
25
distance
2.5. Selection of the useful limits of the welding parameter:
Trial runs were carried out by varying one of the process parameters whilst keeping the rest of them at constant
values. The working range was decided upon by inspecting the bead for smooth appearance and the absences of
any visible defects. The upper limit of a factor was coded as +1 and lower limit as -1. The selected process
parameters with their limits, units and notation are given in Table.1 above.
2.6. Developing the design matrix
The designed matrix is given below the level (or signs) for the parameter C (nozzle to plate distance) are
derived by the relation C=V*I*F*S
Table 2. Design matrix
Weld. no
1
2
3
4
5
6
7
8
9
V
volts
-1
-1
-1
-1
-1
-1
-1
-1
-1
ISSN : 0975-5462
I
amp
-1
-1
-1
-1
-1
-1
-1
-1
+1
F
mm/min
-1
-1
-1
-1
+1
+1
+1
+1
-1
S
mm/m
-1
+1
-1
+1
-1
+1
-1
+1
-1
Vol. 3 No.10 October 2011
C*
mm
+1
-1
+1
-1
-1
+1
-1
+1
-1
Treatment
combination+ve
C
S
C
S
F
FSC
F
FSC
I
7410
Shahnwaz Alam et al. / International Journal of Engineering Science and Technology (IJEST)
10
-1
+1
-1
+1
11
-1
+1
-1
-1
12
-1
+1
-1
+1
13
-1
+1
+1
-1
14
-1
+1
+1
+1
15
-1
+1
+1
-1
16
-1
+1
+1
+1
17
+1
-1
-1
-1
18
+1
-1
-1
+1
19
+1
-1
-1
-1
20
+1
-1
-1
+1
21
+1
-1
+1
-1
22
+1
-1
+1
+1
23
+1
-1
+1
-1
24
+1
-1
+1
+1
25
+1
+1
-1
-1
26
+1
+1
-1
+1
27
+1
+1
-1
-1
28
+1
+1
-1
+1
29
+1
+1
+1
-1
30
+1
+1
+1
+1
31
+1
+1
+1
-1
32
+1
+1
+1
+1
The numbers in the first column indicate the number of trial run
+1
-1
+1
+1
-1
+1
+1
-1
+1
-1
+1
+1
-1
+1
-1
+1
-1
+1
-1
-1
+1
-1
+1
ISC
I
ISC
IFC
IFS
IFC
VIFSC
V
VSC
V
VSC
VFC
VFS
VFC
VFS
VIC
VIS
VIC
VIS
VIF
VIFSC
VIF
VIFSC
Table- 3. The observed values of the responces.
Weld.
No
1
2
3
4
5
6
7
8
9
10
11
12
13
14
15
16
17
18
19
20
ISSN : 0975-5462
V
volt
29
29
29
29
29
29
29
29
29
29
29
29
29
29
29
29
35
35
35
35
I
Amp
400
400
400
400
400
400
400
400
550
550
550
550
550
550
550
550
400
400
400
400
F
mm/min
1600
1600
1600
1600
3400
3400
3400
3400
1600
1600
1600
1600
3400
3400
3400
3400
1600
1600
1600
1600
S
mm/min
360
600
360
600
360
600
360
600
360
600
360
600
360
600
360
600
360
600
360
600
Vol. 3 No.10 October 2011
C
mm
30
25
30
25
25
30
25
30
25
30
25
30
30
25
30
30
25
30
25
30
Penetration
(P)mm
2.80
3.16
2.70
3.06
5.11
2.80
5.01
2.70
4.69
4.52
4.59
4.42
4.62
4.61
4.52
4.52
5.50
3.66
5.50
3.56
7411
Shahnwaz Alam et al. / International Journal of Engineering Science and Technology (IJEST)
21
22
23
24
25
26
27
28
29
30
31
32
35
35
35
35
35
35
35
35
35
35
35
35
400
400
400
400
550
550
550
550
550
550
550
550
3400
3400
3400
3400
1600
1600
1600
1600
3400
3400
3400
3400
360
600
360
600
360
600
360
600
360
600
360
600
30
25
30
25
30
25
30
25
25
30
25
30
5.51
5.40
5.41
5.50
8.22
7.49
8.12
7.39
11.48
8.22
11.58
8.12
2.7. Development of mathematical models
Mathematical models can now be developed for the SAW process to predict weld bead penetration and to
establish the interrelationship between welding process parameters to weld bead penetration. The experimental
data were used to develop linear models, and analysis of the models was carried out through ANOVA and
Minitab software was used for this purpose.
The general response function representing any of the weld-bead dimensions can be
Expressed as
Y. = ƒ (V, I, F, S, C)
Where, Y= Weld bead response, V= Open Arc voltage, I= Current=Wire feed rate, S= Welding speed, and
C= Nozzle-to-plate distance.
The effect caused by change in five main factors and their first order interaction can be expressed as the
relationship selected being a first order linear equation
Y=b0+b*V+b2*I+b3*F+b4*S+b5*C+b12*VI+b13*VF+b14*VS++b15*VC+b23*IF+b24*IS+b25*IC+b34*FS
+b35*FC+b45*SC
Where Y represents any of the weld bead dimensions , b0 is constant and b1,b2,b3,b4,b5,b11 ,
b12,b13,b14,b15,b23,b24,b25,b34,b35,b45 are co-efficient of the model.
Signs for calculating effects of parameters and their interactions. The signs for the interaction were obtained by
multiplying the corresponding signs of the involved factors (Table.4)
Table 4. The signs for main and interaction effects.
Trial
no
1
2
3
4
5
6
7
8
9
10
11
12
13
14
X0
V
I
F
S
C
VI
VF
VS
VC
IF
IS
IC
FS
FC
SC
+1
+1
+1
+1
+1
+1
+1
+1
+1
+1
+1
+1
+1
+1
-1
-1
-1
-1
-1
-1
-1
-1
-1
-1
-1
-1
-1
-1
-1
-1
-1
-1
-1
-1
-1
-1
+1
+1
+1
+1
+1
+1
-1
-1
-1
-1
+1
+1
+1
+1
-1
-1
-1
-1
+1
+1
-1
+1
-1
+1
-1
+1
-1
+1
-1
+1
-1
+1
-1
+1
+1
-1
+1
-1
-1
+1
-1
+1
-1
+1
-1
+1
+1
-1
+1
+1
+1
+1
+1
+1
+1
+1
-1
-1
-1
-1
-1
-1
+1
+1
+1
+1
-1
-1
-1
-1
+1
+1
+1
+1
-1
-1
+1
-1
+1
-1
+1
-1
+1
-1
+1
-1
+1
-1
+1
-1
-1
+1
-1
+1
+1
-1
+1
-1
+1
+1
+1
+1
+1
+1
+1
+1
+1
+1
-1
-1
-1
-1
-1
-1
-1
-1
+1
+1
+1
-1
+1
-1
+1
-1
+1
-1
-1
+1
-1
+1
-1
+1
-1
+1
-1
+1
+1
-1
+1
-1
-1
+1
-1
+1
+1
-1
+1
-1
+1
-1
-1
+1
-1
+1
+1
-1
+1
-1
-1
+1
-1
+1
-1
+1
-1
+1
-1
+1
+1
-1
+1
-1
+1
-1
-1
-1
-1
-1
+1
+1
+1
+1
+1
+1
+1
+1
-1
-1
ISSN : 0975-5462
Vol. 3 No.10 October 2011
7412
Shahnwaz Alam et al. / International Journal of Engineering Science and Technology (IJEST)
15
16
17
18
19
20
21
22
23
24
25
26
27
28
29
30
31
32
+1
+1
+1
+1
+1
+1
+1
+1
+1
+1
+1
+1
+1
+1
+1
+1
+1
+1
-1
-1
+1
+1
+1
+1
+1
+1
+1
+1
+1
+1
+1
+1
+1
+1
+1
+1
+1
+1
-1
-1
-1
-1
-1
-1
-1
-1
+1
+1
+1
+1
+1
+1
+1
+1
+1
+1
-1
-1
-1
-1
+1
+1
+1
+1
-1
-1
-1
-1
+1
+1
+1
+1
-1
+1
-1
+1
-1
+1
-1
+1
-1
+1
-1
+1
-1
+1
-1
+1
-1
+1
+1
+1
-1
+1
-1
+1
+1
-1
+1
-1
+1
-1
+1
-1
-1
+1
-1
+1
-1
-1
-1
-1
-1
-1
-1
-1
-1
-1
+1
+1
+1
+1
+1
+1
+1
+1
-1
-1
-1
-1
-1
-1
+1
+1
+1
+1
-1
-1
-1
-1
+1
+1
+1
+1
+1
-1
-1
+1
-1
+1
-1
+1
-1
+1
-1
+1
-1
+1
-1
+1
-1
+1
+1
+1
-1
+1
-1
+1
+1
-1
+1
-1
+1
-1
+1
-1
-1
+1
-1
+1
+1
+1
+1
+1
+1
+1
-1
-1
-1
-1
-1
-1
-1
-1
+1
+1
+1
+1
-1
+1
+1
-1
+1
-1
+1
-1
+1
-1
-1
+1
-1
+1
-1
+1
-1
+1
+1
+1
+1
-1
+1
-1
-1
+1
-1
+1
+1
-1
+1
-1
-1
+1
-1
+1
-1
+1
+1
-1
+1
-1
-1
+1
-1
+1
+1
-1
+1
-1
-1
+1
-1
+1
+1
+1
+1
-1
+1
-1
+1
-1
+1
-1
-1
+1
-1
+1
-1
+1
-1
+1
Table 5. Coefficients of the models
Serial no
Coefficients Bj
1
2
3
4
5
6
7
8
9
10
11
12
13
14
15
16
B0
B1
B2
B3
B4
B5
B12
B13
B14
B15
B23
B24
B25
B34
B35
B45
Penetration
(P)
5.50251
1.41374
1.29126
0.50756
-0.49119
-0.42275
0.61999
0.22869
-0.25756
-0.13480
0.03881
-0.00994
0.14600
-0.22114
-0.24520
0.26605
2.8. Evaluation of the co-efficient of the model
The values of the coefficients of the linear equation were calculated by the regression method. The Minitab and
SPSS software package were used to calculate the values of these coefficients for different responses. All the
coefficients were tested for their significance at 95% confidence level applying student’s t-test.
2.9. Response
Penetration has been expressed as a linear function of the input process
Parameters (in coded form) as follows:
ISSN : 0975-5462
Vol. 3 No.10 October 2011
7413
-1
+1
+1
+1
+1
+1
-1
-1
-1
-1
-1
-1
-1
-1
+1
+1
+1
+1
Shahnwaz Alam et al. / International Journal of Engineering Science and Technology (IJEST)
Y=5.50+1.41*V+1.29*I+0.508*F-0.491*S-0.423*C+0.620*VI+0.229*VF-0.258*VS-0.135*VC+0.0388*IF0.0099*IS+0.146*IC-0.221*FS-0.245*FC+0.266*SC
2.10. Checking adequacy of the model
The analysis of variance (ANOVA) technique has been used to check the adequacy of the developed model.
Analysis of variance tests for models, t-test, p- value, standard error of estimate, coefficient of multiple
correlations, has been estimated and the results are given in Table.6.
Table .6
source
regression
Residual error
total
DF
15
16
31
SS
164.852
0.208
165.060
MS
10.990
0.013
F
844.60
P
0.000
Model name
SEE
R
Penetration
0.1141
.999
99.8
From the above tests it is evident that the model are adequate.
2.11. T- Test for significance of regression coefficients
The determination of co-efficient (R2) indicates the goodness of the fit for the model. In the case of penetration,
the value of the determination co-efficient (R2 = 0.999) indicates the high level of significance. Scatter diagram
between actual and predicted values of reinforcement height has been presented in Fig.3. It can be observed that
there is a good correlation between the actual and predicted values which further supports the validity of
developed model.
2.12. Predicted response: The final mathematical model
Penetration was expressed as a linear function of the input process
Parameters (in coded form) as follow as:
Y=5.50-1.41*V-1.29*I+0.508*F-0.491*S-0.423*C+0.620*VI+0.229*VF-0.258*VS-0.135*VC+0.146*IC0.221*FS-0.245*FC+0.266*SC
Fig.3 Plot of actual vs. predicted response of penetration.
3. Results and discussion:
The predicted influences of the welding parameters on the weld bead penetration within the range of
investigation are shown in Fig.4.and the interaction effects between variables are shown in Fig.5.1 to Fig.5.5.
3.1. Direct effect or main effect of process parameters on penetration:
Figure 4 shows the effect of input parameters on bead penetration in submerged welding process. As shown in
the figure the penetration increases rapidly with increase in voltage and welding current. Significantly increases
with increase in wire feed rate and decreases with welding speed and further significantly decreases with
increase of nozzle to plate distance.
ISSN : 0975-5462
Vol. 3 No.10 October 2011
7414
Shahnwaz Alam et al. / International Journal of Engineering Science and Technology (IJEST)
Fig.4 Main effect plot for penetration.
3.2. Major interaction effect of process parameters on penetration:
It is seen from Fig.5.1 that at high voltage value the penetration rapidly increases with increase in current,
however at low voltage value penetration increase at very slow rate with increase in current. Fig.-5.2 shows that
as the high voltage value the penetration increases with increase in wire feed rate, however at lower voltage
value the penetration increases at very slow rate with increase in wire feed rate. It evident from Fig.-5.3 that the
penetration decreases with increase in welding speed at high voltage value and penetration is very less at low
voltage value ,it is due to that at high welding speed, the heat input per unit length decreases and so penetration
will also decreases. Fig.-5.4 show that as the high wire feed rate, the penetration decreases rapidly with
increases in nozzle to plate distance, however at low wire feed rate the penetration decrease in significantly with
increase in nozzle to plate distance, It is due to resistance heating of the wire before the formation of an arc
which results in higher metal deposition rate owing to higher heat input. Fig.-5.5 show that as the low welding
speed , the penetration decreases rapidly with increases in nozzle to plate distance, however at high welding
speed the penetration decreases insignificantly with increase in nozzle to plate distance.
Fig.5.1
Fig.5.2
Fig.5.4
4.
Fig.5.3
Fig.5.5
Conclusions
 The two level full factorial designs are found to be an effective tool for quantifying the main and
interaction effect of variables on weld bead penetration.
ISSN : 0975-5462
Vol. 3 No.10 October 2011
7415
Shahnwaz Alam et al. / International Journal of Engineering Science and Technology (IJEST)

The developed model can be effectively used to predict the penetration in the submerged arc welding
within the range of parameters used.
 Proposed models are adequate to predict with confidence level of 95%.
 Penetration increase significantly with increase in voltage, current and wire feed rate .decrease with
increase in welding speed and nozzle to plate distance.
References
[1]
[2]
[3]
[4]
Howard Carry B, Modern Welding Technology,(Prentice Hall Inc, Englewood Cliffs,NJ), 1979
Nadkarni S V, Modern Welding Technology, (Oxford &amp;IBH Publishing Co. Pvt Ltd, New Delhi).1988
Houldcroft, P. T. 1989. Submerged Arc Welding. Abington, U.K
D. Kim, M. Kang, S. Rhee, Determination Of Optimal Welding Conditions With A Controlled Random Search Procedure, Welding
Journal 8 (2005) 125-130.
[5] J. Raveendra, R.S. Parmar, Mathematical Models To Predict Weld Bead Geometry For Flux Cored Arc Welding, Metal Construction
19/2 (1987) 31-35.
[6] L.J. Yang, R.S. Chandel, M.J. Bibby, The Effects Of Process Variables On The Weld Deposit Area Of Submerged Arc Welds,
Welding Journal 72/1 (1993) 11-18.
[7] R.S. Chandel, H.P. Seow, F.L. Cheong, “Effect Of Increasing Deposition Rate On The Bead Geometry Of Submerged Arc Welds”
,Journal of Materials Processing Technology.72 (1997)124 – 128.
[8] S. Datta, M. Sundar, A. Bandyopadhyay, P.K. Pal, S.C. Roy, G. Nandi, Statistical Modeling For Predicting Bead Volume Of
Submerged Arc Butt Welds, Australasian Welding Journal 51/2 (2006) 39-47.
[9] Gupta and Parmar ,Fractional Factorial Technique To Predict Dimensions Of The Weld Bead In Automatic Submerged Arc Welding ,
J Inst Engr (India), 70 (1986) 67-71
[10] Ravindra J&amp; Pramar R S , Mathematical Model To Predict Weld Bead Geometry For The Flux Cored Welding Process, Metal
Construct, 19 (1987) 31 R-35R
ISSN : 0975-5462
Vol. 3 No.10 October 2011
7416
```